- Home
- Documents
- Modeling and experimental study of birefringence in injection molding of semicrystalline polymers

prev

next

out of 21

Published on

26-Jun-2016View

218Download

3

Transcript

bi

lin

, K

iversit

line 8

s E. M

s is v

ow-in

n the

glass transition temperature. In semicrystalline polymers,of the polymer during the non-uniform cooling through a

Polymer 46 (2005)E-mail address: aisayev@uakron.edu (A.I. Isayev).induced crystallization occurred. The flow effect on the equilibrium melting temperature elevation due to the entropy reduction between the

oriented and unoriented melts was incorporated to model crystallization. To find the entropy reduction and the frozen-in elastic recovery

during crystallization, a non-linear viscoelastic constitutive equation was used. From the ultimate elastic recovery the crystalline orientation

function was calculated. The crystalline and amorphous contributions to the overall birefringence were obtained from the crystalline

orientation function and the flow birefringence, respectively. The birefringence profiles were measured and predicted in moldings of

polypropylenes of different molecular weights obtained at various melt temperatures, injection speeds, holding times and mold temperatures.

The resulting predictions were in fair agreement with corresponding experimental data.

q 2005 Elsevier Ltd. All rights reserved.

Keywords: Viscoelastic; Birefringence; Injection molding

1. Introduction

The properties of polymer products are closely related to

their morphology, resulting from the mechanical and

thermal history experienced during the manufacturing

process. Upon the imposition of deformation or strain,

polymer melt flows and accumulates both the elastic and

plastic strains due to the viscoelastic nature of polymer

molecules. Polymer molecules are extended in the flow

direction. The molecular orientation due to flow depends on

the value of elastic part of the total strain. Upon the

cessation of flow, the orientation reduces as the elastic strain

decreases.

In amorphous polymers [1], the elastic strain or

orientation freezes when the temperature goes below the

temperature. The frozen-in orientation is related to the

birefringence, because the molecular orientation increases

the polarizability along the molecular chain.

In processing operations, such as the injection molding or

extrusion, frozen-in orientations and residual stresses arise

[2]. The flow-induced stresses arise from the shear and

normal stresses during flow, leading to the orientation of

polymer chains. If these stresses and orientations do not

completely relax during the subsequent cooling period, they

appear as the frozen-in birefringence and flow stresses in the

products. In case of the injection molding, the extensional

flow at a melt front also causes birefringence.

Residual thermal stresses arise due to the differential

density or shrinkage variation and the viscoelastic behaviorModeling and experimental study of

semicrystal

Kyuk Hyun Kim, A.I. Isayev*

Institute of Polymer Engineering, The Un

Available on

This article is dedicated to Professor Jame

Abstract

The prediction of birefringence developed in injection molding

products. A novel approach for the numerical simulation of the fl

semicrystalline polymers was proposed. The approach was based orefringence in injection molding of

e polymers

eehae Kwon, C. van Sweden

y of Akron, Akron, OH 44325-0301, USA

March 2005

ark on the occasion of his 70th Birthday

ery important in order to satisfy required specification of molded

duced crystallization and frozen-in birefringence in moldings of

calculation of elastic recovery that becomes frozen when the flow-

41834203

www.elsevier.com/locate/polymerwhen it vitrifies or crystallizes. The coupling between these

various stresses occurs during cooling and annealing. The

degree of coupling appears to depend on the molecular

conformation and is not yet completely understood. The

frozen-in strains and stress patterns in injection molded0032-3861/$ - see front matter q 2005 Elsevier Ltd. All rights reserved.

doi:10.1016/j.polymer.2005.02.057

* Corresponding author. Tel.:C1 330 972 6673; fax:C1 330 258 2339.this condition may be reached below the crystallizationglass transition or a crystallization temperature. Thermal

birefringence arises due to viscoelastic behavior of polymer

pa

she

ment of birefringence [1317]. Typically predicted birefrin-

gence development does not coincide with the

rC

wh

Cp

K.H. Kim et al. / Polymer 46 (2005) 418342034184experimentally measured birefringence.

In the present study, the numerical simulation of the

flow-induced crystallization and frozen-in birefringence in

moldings of semicrystalline polymers was carried out. The

approach was based on the calculation of the elastic strain

that becomes frozen at the onset of crystallization. The flow

effect on the equilibrium melting temperature elevation due

to the entropy reduction between the oriented and

unoriented melts was incorporated to model crystallization

[17,18]. To find the frozen-in elastic recovery during

crystallization and entropy reduction, a non-linear viscoe-

lastic constitutive equation was used. From the elastic

recovery the crystalline orientation function was calculated

by using Gaylords theoretical analysis [19]. Then crystal-

line and amorphous contributions to the overall birefrin-

gence were obtained from the crystalline orientation

function and the flow birefringence, respectively.

2. Theoretical consideration

2.1. Governing equations

The melt delivery system and mold cavity are typically

comprised of the geometric elements having either circular

or rectangular cross section. Along the flow channel,

geometric discontinuity occurs at the gate and junctures.

The physical nature of the flow during the injection molding

process in the channel allows for some simplifications of the

governing transport equations for the non-isothermal flow of

non-Newtonian fluids.

These may be summarized as follows:

1. The lubrication approximation is introduced. Due to

small Reynolds number, inertia forces are neglected. In

addition, the velocity and dynamic forces in the gapwisedirectly [25]. However, since the flow stresses give rise to

the molecular orientation, the measurement of frozen-in

molecular orientation in terms of residual birefringence is

an indirect indication of the residual flow stresses. That is, a

distribution of flow stresses in moldings can be constructed

from the birefringence measurement by the use of rheo-

optical rule, relating the residual birefringence and flow

stresses. This has been found to be generally true for

amorphous polymers [27]. There are also a few attempts

made to theoretically predict the residual flow stresses and

correlate them with the measured frozen-in birefringence

[25,812]. However, for the case of semicrystalline

polymers, little information is available, related to the

prediction of crystallization and its effect on the develop-rts are more complex than those in extruded films or

ets.

In general, residual flow stresses cannot be measuredor radial direction are neglected along with the temere r is the density, u is the velocity in the flow direction,

is the specific heat capacity, P is the pressure, T is theZr vr

rvr

CF

C _Q cylindrical coordinates (5)p

vT

vtCu

vT

vx

k v vT Zextensional flow arising in juncture region of mold and

elongational flow at the melt front.

2. The polymer melt is assumed to be viscoelastic with the

behavior obeying Leonov model [20], which incorpor-

ates temperature, time and shear rate dependence.

3. The compressibility of polymer melt, which is important

during the packing stage, is taken into account by

SpencerGilmore PVT equation of state [2123]. How-

ever, without the loss of accuracy, the incompressibility

of the melt is assumed during the filling stage.

4. Heat conduction is limited to the gapwise direction of a

flow channel, with polymer temperature at a wall being

set to that of a mold, Tw. Besides, heat convection is

considered only along the flow direction.

The assumptions and simplifications stated above lead to

HeleShaw type flow of the polymer melt, according to

which the pressure is independent upon the gapwise (or

radial) location.

The 1-D flow in a rectangular channel having the

gapwise thickness of 2b and the width of W is considered. In

addition, the flow in a tube having the radius of R is

considered. The Cartesian coordinate system is defined such

that the flow direction is designated as x-axis and the

gapwise direction as y-axis. In cylindrical coordinates, the

radius direction is designated as r-axis. The governing

transport equations are:

Equation of continuity:

vr

vtCvruvxZ 0 (1)

Equation of motion:

vP

vxC

v

vyhvu

vy

Z 0 Cartesian coordinates (2)

vP

vxC

1

r

v

vrhrvu

vr

Z 0 cylindrical coordinates (3)

Equation of energy conservation:

rCpvT

vtCu

vT

vx

kv2T

vy2CFC _Q Cartesian coordinates (4)perature, k is the thermal conductivity of the polymer, h

t Z Z h _g cylindrical coordinates (24)

mer 4is the viscosity, F is the energy dissipation and _Q is the rateof heat release due to crystallization per unit volume.

The rate of heat release due to crystallization is defined

according to the crystallization kinetics as follows:

_QZ rXNDHcdq

dt(6)

where XN is the ultimate degree of crystallinity, DHc is theheat of fusion per unit mass for the pure crystal and q is the

relative degree of crystallinity.

For a viscoelastic flow, the energy dissipation function is

[24]:

FZ 2sh0 tr E2

CXNkZ1

hk

4q2k

IkCIIkCK IkC3

C trC2ij;kK3

(7)

where E is the deformation-rate tensor, s is the dimension-less rheological parameter lying between zero and unity, h0is the zero-shear-rate viscosity, hk is the shear viscosity of

the kth mode, IkC and IIkC are the first and the second invariant

of the elastic strain tensor, Cij,k, and qk is the relaxation time.

Leonov multi-mode non-linear constitutive equation was

used to describe the rheological behavior of polymer melts

[20]:

CVij;kC1

2qkC2ij;kC 1

3IIkCK IkCCij;kK IZ 0 (8)

where I is the identity tensor and CVij;k is the Jaumannderivative.

The deformation-rate tensor and the zero-shear-rate

viscosity may be expressed as

EZ1

2fV uC V uTg (9)

h0TZPN

kZ1 hkT1Ks

(10)

The viscosity and the relaxation time are assumed to

have an Arrhenius-type temperature dependence:

hkTZAk exp TbT

(11)

qkTZBk exp TbT

(12)

where Tb is the temperature sensitivity related to the

activation energy and Ak, Bk are constants.

These values may increase dramatically as the polymer

crystallizes. However, the crystallinity effect on the

viscosity and relaxation time was not considered in this

study.

In case of simple shear, the elastic strain tensor has the

K.H. Kim et al. / Polyfollowing form:Cij;kZ

C11;k C12;k 0

C12;k C22;k 0

0 0 1

264

375 (13)

For 1-D incompressible case in the filling stage, the

conservation of mass and momentum may be expressed as

[2]:

v

vxSvP

vx

Z 0 (14)

where fluidity S is defined as:

SZ

b0

y2

hdy Cartesian coordinates (15)

SZ1

2

R0

r3

hdr cylindrical coordinates (16)

The average velocity, u, can be expressed as

uZ1

b

b0

u dy Cartesian coordinates (17)

uZ2

R2

R0

ru dr cylindrical coordinates (18)

According to the N-mode Leonov model, the stress

tensor tij is then given by:

tijy; tZ 2mq1Ts _g0 1 0

1 0 0

0 0 0

264

375

C2XNkZ1

mkTC11;k C12;k 0

C12;k C22;k 0

0 0 1

264

375 (19)

where _gZKvu=vy is the shear rate, mkZhk/2qk is themodulus of kth mode and mZh0/2q1.

The governing equation for Cij,k in Eq. (8) can be

expressed in the component form as:

DC11;k

DtK2C12;k

vu

vyC

1

2qkC211;kCC212;kK1Z 0 (20)

DC12;k

DtKC22;k

vu

vyC

1

2qkC11;kCC22:kC12;kZ 0 (21)

C11;kC22;kKC212;kZ 1 (22)

with D/Dt being the material derivative operator.

Introducing the pressure gradient, L, the shear stress, t12,

can be expressed by:

t12ZLyZ h _g Cartesian coordinates (23)

Lr

6 (2005) 41834203 4185122

mer 4On the other hand, by integrating Eq. (17) (Cartesian) or

Eq. (18) (cylindrical) by part, and eliminating _g using Eq.(23) (Cartesian) or Eq. (24) (cylindrical), it follows:

uZL

b

b0

y2

hdyZ

L

bS Cartesian coordinates (25)

uZL

R2

R0

r3

2hdrZ

LS

R2cylindrical coordinates (26)

Accordingly, from Eqs. (17), (19), (23) and (25) for

Cartesian coordinates, or from Eqs. (18), (19), (24) and (26)

for cylindrical coordinates, L can be expressed as

LtZ2msb uK2

PNkZ1 mk

b0

yC12;kq1

dy

b0

y2

q1dy

Cartesian coordinates

(27)

LtZ4msR2 uK4

PNkZ1 mk

R0

r2C12;kq1

dr

R0

r3

q1dr

cylindrical coordinates

(28)

The elastic strain tensor components at a steady state

flow, Cstij;k, can be expressed by:

Cst11;kZ

2

pXk

1CXkp (29)

Cst12;kZ2 _gXk1CXk

(30)

Cst22;kZ

2

p1CXk

p (31)

where XkZ1C1C4 _gqk2

p.

The shear viscosity can be expressed as

hZ h0sCXNkZ1

2hk

1C1C4 _gqk2

p (32)In order to consider the compressibility during the packing

stage, SpencerGilmore thermodynamic equation of state

[2123] can be used as:

P P1rK

1

r R^T (33)

The specific volume for semicrystalline polymers can be

calculated from Eq. (33) as:

VT ; P 1rT ; P

1

r R

P P T 1

rt(34)

where a typical PVT curve is comprised of two linear

regions of rubbery and glassy state separated at the glass

transition temperature including the density compensation

term, rt, to handle the sharp density change in the vicinity ofcrystallization temperature, Tt as proposed in [25]. Material

K.H. Kim et al. / Poly4186constants, r; R; P, are different for the rubbery and glassystates. They can be determined from two separate fits to

experimental data.

Eq. (34) can be expressed in two separate regions as

follows:

if TRTt

1

rtZ b7 expb8 TKb9P; rZ rl; RZ Rl; PZ Pl (35)

if T!Tt

1

rtZ 0; rZ rs; RZ Rs; PZ Ps (36)

with

Tt b5 b6P and T TKb5 (37)where b5, b6, b7, b8, b9, and, rl; Rl; Pl and rs; Rs; Ps arefitted material parameters at the above and below the phase

transition temperature for semicrystalline polymers.

For a semicrystalline polymer like PP, a typical PVT

curve consists of two linear regions of the rubbery and

glassy state with a transition zone in between. The specific

volume at the transition region as a function of crystallinity

as well as temperature and pressure is calculated by:

VT ; P; XcZXcVsT ; PC 1KXcVlT ; P (38)where Vl and Vs are the specific volume above and below the

transition temperature and Xc is the absolute degree of

crystallinity.

Since the specific volume depends on the pressure and

temperature one can write:

vr

vtZ

vr

vP

T

vP

vtC

vr

vT

P

vT

vt(39)

where

vr

vP

T

Zr

PC P^1Krr^

(40)

vr

vT

P

ZKr

T1Krr^

(41)

Assuming no slip condition at the mold wall and the

geometric symmetry of the flow channel, appropriate

boundary conditions for the velocity and temperature

could be specified as follows:

ujyZb; yZRZ 0; vuvy

jyZ0Z 0 (42)

TjyZb; yZRZ Tw; vTvy

jyZ0Z 0 (43)

Since pressure P is assumed to be independent of y-

position, the integration of Eq. (2) over y (Cartesian) or Eq.

(3) over r (cylindrical), with the incorporation of Eq. (42),

6 (2005) 41834203gives:

LZKvx

(46)

difference between the heat released by crystallization,

mer 4Further, by integrating Eq. (44) (Cartesian) or Eq. (45)

(cylindrical) and making use of Eq. (42), one can get:

uZL

by

y

h

dy Cartesian coordinates (47)

uZL

Rr

r

2h

dr cyli...